• date post

06-Jun-2020
• Category

## Documents

• view

6

0

Embed Size (px)

### Transcript of Dimensional analysis - zeus.plmsc.psu.edu manias/MatSE447/23-26_ Dimensional analysis EXAMPLE: FLOW...

• Dimensional analysis The Buckingham π Theorem - If there are m physical quantities con-

taining r fundamental units, then there are π = m− r dimensionless groups that are independent.

Procedure: 1. Write down all relevant physical quantities and their fundamental units. 2. Determine π. 3. Write down the π dimensionless groups.

Example: Flow through a circular pipe

dP

dx = f(Q, R, µ) m = 4

dP

dx

( dynes

cm3 =

g

cm2s2

) Q (cm3/s)

R (cm)

µ

( dynes

cm2 s =

g

cm s

) g, cm, s r = 3

∴ π = m− r = 1

1

µ

dP

dx

( 1

cm s

) only way to get rid of grams

1

µQ

dP

dx

( 1

cm4

) only way to get rid of seconds

R4

µQ

dP

dx (dimensionless)

Dimensional Analysis ⇒ dP dx ∼ µQ

R4

1

• Dimensional analysis

Dimensional Analysis ⇒ dP dx ∼ µQ

R4

Not as useful as the exact result:

∆P

L =

8

π

µQ

R4

because exact result has the prefactor.

How did we get so much information? We cheated!

Used “experience” to guess that ∆P and L would only enter as dP/dx = ∆P/L, and that the velocity v would only enter though Q.

“Honest” Treatment:

∆P = f(Q,R,L, µ, v)

∆P (g/cm s2)

Q (cm3/s)

R (cm)

L (cm)

µ (g/cm s)

v (cm/s)

m = 6 r = 3 ∴ π = m− r = 3

2

• Dimensional analysis EXAMPLE: FLOW IN AN EXTRUDER

dP

dx = f(Q, Ds, hs, Ns, φs, µ)

( g cm2s2

) Q (cm3/s) volumetric flow rate

Ds (cm) barrel diameter

hs (cm) flight depth

Ns (1/s) screw rotation rate

φs (dimensionless) helical angle of screw

µ (g/cm s) viscosity

m = 7, r = 3 ⇒ π = m− r = 4

Four dimensionless groups

φs, Ds hs

, Q

NsD3s

1

µ

dP

dx

( 1

cm s

) (cancels grams)

Ds µNs

dP

4

• Dimensional analysis EXAMPLE: FLOW IN AN EXTRUDER

Ds µNs

dP

dx = f

( φs, Ds/hs, Q/(NsD

3 s)

) Optimum φs = 23

◦ (universally utilized) Most extruders are geometrically similar and designed to provide a certain

pressure at the die:

∴ Ds hs ∼= constant

∴ Ds µNs

dP

dx ∼= constant

If other three dimensionless groups are constant, then the last one must also be constant.

Expect Q ∼ NsD3s (not obvious)

5

• Melt Fiber-Spinning

1

• Melt vs. Solution Fiber-Spinning

2

• PIPE EXTRUSION: Die Swell is Crucial!

Mandrel Supports:

1

• Profile Extrusion

3

• Sheet Processing SHEET EXTRUSION

1

• Sheet Processing CLAM SHELLING IN A SHEET DIE

Figure 1: Pressure is very high (100atm) at the center of the die.

Figure 2: High pressure causes die to creep. After extensive extrusion, sheet will be thicker in the center.

2

• Sheet Processing POST-DIE SHEET FORMING

Calendering Thin Sheet:

3

• COEXTRUSION LAYER PACKS

9

• COEXTRUSION BARRIER POLYMERS

EVOH (ethylene-vinyl alcohol) random copolymer with 30%E PVDC (polyvinylidene chloride) [CH2CCl2]

8

• COEXTRUSION

5

• COEXTRUSION

6

• COEXTRUSION

7

• FILM BLOWING

3

• FILM BLOWING

4

• P rofile

E xtru

sion

2

• Wire Coating

Combination of Poiseuille flow (pressure driven) and Couette (drag) flow due to the moving wire.

First we do the Couette Flow problem assuming ∆P = 0.

vr = vθ = 0 vz = vz(r) dP

dr =

dP

dθ =

dP

dz = 0

Continuity is identically satisfied

N.-S.: µ 1

r

d

dr

( r dvz dr

) = 0

d

dr

( r dvz dr

) = 0 r

dvz dr

= C1

dvz dr

= C1 r

vz = C1 ln r + C2

5

manias Text Box More on Wire-Coating in the NEXT LECTURE

• Sheet Processing THERMOFORMING

R.G. Griskey, Polymer Process Engineering, chapter 10

J. Florian, Practical Thermoforming (Marcel Dekker, 1987)

Extrude a Sheet, Clamp it, Heat it up, and ...

4

• THERMOFORMING VACUUM FORMING

∆P = 1atm.

5

• THERMOFORMING VENTING

6

• THERMOFORMING PRESSURE-ASSISTED

To exceed ∆P = 1 atm. use pressurized air.

Avoid trapped air by using vacuum.

7